Removal of Cr(vi) in wastewater by Fe–Mn oxide loaded sludge biochar

Sludge biochar loaded with Fe–Mn oxides (FMBC) was prepared and employed to remove Cr(vi) from wastewater. The influences of solution pH, co-existing ion, contact time, adsorption temperature and Cd(vi) concentrations on removing Cr(vi) by FMBC were investigated. The Cr(vi) adsorption on FMBC had strong pH dependence. Additionally, Na+, Mg2+, Ca2+, SiO32−, NO3− and Cl− ions exhibited no influence on Cr(vi) removal efficiency for FMBC, whereas there were inhibition effects of Pb2+, Cu2+, Ni2+, CO32−, SO42−, and PO43− on removing Cr(vi). The Cr(vi) adsorption from solution for FMBC was well described by models of pseudo-second-order and Langmuir, and the largest Cr(vi) removal capacity of FMBC reached 172.3 mg g−1. FMBC had good capacity for treating electroplating wastewater and mineral dissolving wastewater containing Cr(vi). After five regenerations, the 50 and 5 mg L−1 Cr(vi) removing efficiency of FMBC was 82.34% and 97.68%, respectively. The Cr(vi) removal for FMBC involved adsorption-reduction and re-adsorption of Cr(iii) generated by reduction. These results indicated that FMBC has good prospects for remediating Cr(vi)-containing wastewater.


Introduction
Chromium (Cr) mainly exists in two valence states, Cr(VI) and Cr(III), of which Cr(VI) is highly toxic, difficult to biodegrade and easy to be enriched in the food chain. 1,2If Cr-containing wastewater is not treated properly, it will bring great harm to human beings and nature.Currently, the main method for Cr(VI) removal is reverse osmosis, ion exchange, oxidation reduction, membrane separation and adsorption. 3Adsorption is considered to be a preferred method for treating Cr(VI) in wastewater because of its simplicity, low cost and high efficiency. 4,5Therefore, research and development of an economical, simple and efficient new adsorbent is of high application value.
7][8] However, the physicochemical properties of biochar, such as surface functional groups, porosity and specic surface area, have great inuence on removing Cr(VI). 6,9Therefore, the Cr(VI) removal effect on biochar in water can be improved by modifying its physicochemical properties and surface structure.Previous literature showed that iron oxides increased the positive charge of biochar and its electrostatic attraction with anionic pollutants was enhanced. 10,11While manganese oxides hold chemically stable and rich -OH functional groups, it is an adsorbent material for efficient adsorption of contaminants in solution. 12owever, in practical applications, the iron and manganese oxides exhibit insufficient mechanical strength, poor occulation and easy agglomeration. 13Biochar as a carrier could effectively improve the agglomeration of Fe-Mn oxides.Aer the introduction of Fe-Mn oxides, the amount of active site of biochar increased, and its removal performance for contaminants was greatly improved. 14Additionally, the multi-metal materials have synergistic adsorption and reduction effects, which can improve the effect of Cr(VI) treatment. 13Applying composites to treat Cr(VI)-containing wastewater is expected to achieve the dual purpose of waste biomass resource utilization and Cr(VI) pollutant control.
Hence, sludge biochar loaded with Fe-Mn oxides (FMBC) was employed to remove Cr(VI) from wastewater.The intentions of this research were to: (i) investigate removal performance of FMBC for Cr(VI) in solution, (ii) elucidate the adsorption mechanism of Cr(VI) by FMBC, and (iii) validate potential of FMBC for remediating electroplating wastewater and mineral dissolving wastewater containing Cr(VI).
Sinopharm Chemical Reagent Co. Ltd (Shanghai, China).Above reagent was of analytical reagent.Different concentration of Cr(VI) solutions was obtained through K 2 Cr 2 O 7 solids dissolution.Dewatering sludge from Chengdu (Sichuan Province, China) municipal wastewater treatment plant.

Preparation of Fe-Mn oxide loaded sludge biochar
Air-dried dry sludge was ground into powder by ball mill.Five gram powdered dry sludges were incorporated into 100 mL deionized water and homogenously stirred for 60 min.Meanwhile, 2 g of FeCl 3 $6H 2 O and 2 g of MnCl 2 $5H 2 O were incorporated into 100 mL deionized water.Above two solutions were added to 500 mL conical ask and solution pH was adjusted to 10-11.0 by 0.1 mol L −1 NaOH solution.Subsequently, suspension shake in a 25 °C thermostatic oscillator at 120 rpm for 12 h.And then, the solution was ltered through a 0.23 mm lter membrane and the solids on membrane were assembled.Then, solids were dried in a thermostatic oven at 80 °C for 12 h.Thereaer, 5 g solid was placed on a ceramic boat and the boat was pyrolyzed in a muffle furnace with N 2 atmosphere at 450 °C for 2 h.Aer pyrolysis, the black solid on the boat was washed with ultrapure water and anhydrous ethanol for 3 times, and the obtained black solid was dried in a constant temperature oven at 80 °C for 12 h.The dried black solid was stored in a sealed bag and recorded as FMBC.

Batch adsorption experiment
Adsorption experiment performed in 100 mL polyethylene centrifuge tube containing 50 mL of Cr(VI) solution.The solution pH was adjusted by 0.1 mol L −1 HNO 3 or NaOH.During the reaction, the centrifuge tubes was set into a shaker at 25 °C and shaken at 150 rpm for 300 min.The effect of pH and co-existing ion on removing Cr(VI) was researched.
Adsorption isotherm: 0.4 g L −1 adsorbent was added to Cr(VI) solution at concentrations of 50-150 mg L −1 , and then solution pH set to 3.0.The suspension was placed into a temperaturecontrolled shaker at multiple temperature (288 K, 298 K and 308 K) to reaction for 300 min.Langmuir, Freundlich, Temkin and Sips model was employed to analyze experimental result (ESI †).
Adsorption kinetics: series of centrifuge tubes containing 50 mg L −1 Cr(VI) solution were set up according to the adsorption time, and 0.4 g L −1 of adsorbent was added to the tubes.The solution pH was set to 3.0, and then adsorption experiment was carried out for 5-300 min in a thermostatic oscillator at 25 °C.The data was analyzed by pseudo-rst-order kinetic model, pseudo-second-order kinetic model, Elovich model, intraparticle diffusion model and liquid lm diffusion model, respectively (ESI †).
To explore practicality of FMBC, Cr(VI) removal experiments were carried out in electroplating wastewater and mineral dissolving wastewater.The content of Cr(VI) in electroplating wastewater and mineral dissolving wastewater were 40.21 and 1.35 mg L −1 , respectively.Since pH of mineral dissolving wastewater was 6.76, the mixed solution pH of mineral dissolving wastewater and adsorbent was adjusted to 3.0 before adsorption.Adsorbent was added to 50 mL electroplating wastewater or mineral dissolving wastewater, and the mixed solution was transferred to oscillator at 25 °C and 150 rpm to adsorb 300 min.The electroplating wastewater came from Baohe swan electroplating plant (Chengdu, China) and mineral dissolving wastewater originated during the construction of railway tunnels in southwestern China.The properties of electroplating wastewater and mineral dissolving wastewater were displayed in Table S1.† Repeatability experiments: 50 mg L −1 Cr(VI) solutions and 0.4 g L −1 absorbent were added into a centrifuge tube, and pH of suspension was set to 3.0.Then suspension was transferred to a oscillator at 25 °C and 150 rpm to adsorb for 300 min.Aer reaction, the solution was ltered, and the absorbent was collected on a nylon lter membrane.The sample was mixed with 0.1 mol L −1 NaOH, and suspension pH was probably around 10.0.The suspensions were shaken in oscillator (25 °C and 150 rpm) for 12 h.Then suspension was ltered through 0.45 mm nylon membrane lter and rinsed with ultrapure water until the rinsing solution was neutral, and samples were dried at 80 °C for 12 h.Repeatability experiment was repeated for 5 times with the regenerated absorbent and Cr(VI) adsorption performances by FMBC for each regeneration were calculated.
The total Cr contents of residual liquid were determined through an inductively coupled plasma optical emission spectrometer (ICP-OES, FL1008M018, Cary, USA).The Cr(VI) contents were determined through modied 1,5-diphenylcarbazide method. 10The Cr(III) content was calculated by content difference between the total Cr and Cr(VI).The removal efficiency (eqn (1)) and adsorption capacity (eqn (2)) were counted.
where R is the removal efficiency, %; C 0 is the initial Cr(VI) concentration, mg L −1 ; C e is the Cr(VI) concentration aer adsorption equilibrium, mg L −1 ; q e is the Cr(VI) adsorption capacity of the adsorbent, mg g −1 ; V is the solution volume, L; and m is the mass of the adsorbent, g.

Characterization analysis
BC and FMBC surface morphology structure was illustrated in Fig. S1.† The surface of BC was smooth and at as shown in Fig. S1a.† Nevertheless, the Fig. S1b † showed the presence of ower-like structure on the FMBC surface, which indicated that Fe-Mn compounds were successfully loaded on sludge biochar surface.According to EDS analysis, the content of Fe and Mn on the FMBC surface was higher than that of BC.Furthermore, Fig. S1c † showed that Fe and Mn were dispersed on FMBC surface, which also indicated that Fe-Mn oxide was loaded on FMBC surface.
The N 2 adsorption-desorption curves of BC and FMBC are displayed in Fig. 1a.Adsorption capacity of N 2 by BC and FMBC gradually increased with increasing relative pressure P/P 0 and a hysteresis loop was formed, which suggested that N 2 adsorption-desorption curves for BC and FMBC was categorized as type IV isotherm. 10,15The non-coincidence in the second half of the adsorption-desorption curves attributed to multilayer lling inuence of capillary pore, suggesting that both micropores and mesopores existed in BC and FMBC, but the material was mainly mesoporous. 16The specic surface area of BC and FMBC was calculated as 25.28 m 2 g −1 and 67.34 m 2 g −1 , respectively.The pore width of BC and FMBC is displayed in Fig. 1b.The pore widths were concentrated in 2-50 nm, which suggested that BC and FMBC were mesoporous material. 3oreover, the average pore size of BC and FMBC was calculated as 9.43 nm and 15.60 nm by methods, respectively.
As shown in Fig. 1c, the Raman shi at 1358 cm −1 and 1595 cm −1 was denoted as D peak and G peak, respectively. 10he I D /I G ratio of BC and FMBC was calculated to be 0.98 and 1.02, respectively, and this result indicated that the graphitization of sludge biochar decreased aer loading with Fe-Mn oxides.Furthermore, FMBC exhibited a new vibrational peak at 658 cm −1 , which was considered to be the characteristic peak of MnFe 2 O 4 . 17The crystalline structures in BC and FMBC were investigated through XRD technique and result are displayed in Fig. 1d.In XRD plot, the main substances in BC and FMBC were SiO 2 and CaAl 2 Si 2 O 8 , which was in agreement with previous ndings. 10,18Moreover, the characteristic peak of Fe 2 O 3 was detected in BC.Notably, new characteristic peaks in FMBC appeared at 2q = 29.86°,35.14°and 61.92°, which was speculated that the new characteristic peaks may be caused by MnFe 2 O 4 . 19In the FTIR prole of BC and FMBC (Fig. 1e), the broad band observed at 3300-3500 cm −1 was related to O-H stretching vibration, and characteristic peak at 1620 cm −1 corresponded to the vibration of C]C/C]O deformation conjugation vibration. 9The vibrational peak appearing at 1430 cm −1 was considered to be due to the -COOH group, while the vibrational peak at 1070 cm −1 was considered to be due to the C-O group. 20Notably, the intensity of O-H, C]C/C]O, and -COOH groups on FMBC were all enhanced upon loading of Fe-Mn oxides, suggesting that the Fe-Mn oxide loading increased the number of O-containing groups in the adsorbents. 13Additionally, the vibrational peak at 531 cm −1 corresponded to Fe-O group in BC. 19 Aer Fe-Mn oxide loading, the characteristic peak at 531 cm −1 was shied to 539 cm −1 , which may be caused by Fe/Mn-O characteristic peak formed by Fe-Mn oxide loading. 19ccording to the full spectrum analysis by XPS (Fig. 1f), the elements C, O, N and Fe appeared in the full XPS spectrum of BC, while the element Mn was found in FMBC.In the O 1 s proles of BC (Fig. S2a †) and FMBC (Fig. S2b †), O 1 s could be classied into M-O (M denoted Fe or Mn), C]O and C-O characteristic peaks.Aer loading Fe-Mn oxides, the relative contents of Fe-O/Mn-O and C]O in FMBC increased from 6.04% and 0.72% to 21.68% and 3.02%, respectively, which demonstrated that Fe-Mn oxides effectively increased the number of O-containing groups on FMBC. 13In Fe 2p prole of BC (Fig. S2c †), The element Fe in BC existed as Fe(III) corresponding to binding energies of 711.07 eV and 724.57eV. 21This was consistent with the results of the XRD analyses.Nevertheless, elemental Fe in FMBC (Fig. S2d †) was present in the form of both Fe(II) and Fe(III), and the relative contents of Fe(II) and Fe(III) were 44.74% and 55.26%, respectively. 21No characteristic peaks were detected in the ne XPS mapping of high-resolution Mn 2p in BC (Fig. S2e †).In Fig. S2f, † a distinct Mn 2p characteristic peak appeared in FMBC, and Mn 2p peaks existed in both Mn(II) and Mn(III) valence states. 12The binding energies of Mn(II) and Mn(III) in the Mn 2p peaks were 640.76/652.28eV and 642.72/653.88eV, respectively, and the relative contents of Mn(II) and Mn(III) were 64.28% and 35.72%, respectively. 12The above analyses demonstrated that the loading of Fe-Mn oxides provided developed pore structure and more O-containing groups for FMBC.

Inuence of solution pH and co-existing ion on removing Cr(VI)
Solution pH is one of crucial factor affecting contaminant removal capacity by absorbent.The result indicated that solution pH obviously (p < 0.05) affected Cr(VI) adsorption performance for FMBC (Fig. 2a and b).The Cr(VI) adsorption capacities for FMBC were approximately 117 mg g −1 at solution pH of 2.0 and 3.0, while Cr(VI) adsorption capacity by FMBC decreased to 1.03 mg g −1 with increasing solution pH to 10.0.The adsorption capacity of Cr(VI) by BC was considerably lower compared to FMBC (Fig. S3 †).The Cr(VI) adsorption capacities for BC were about 63 mg g −1 at solution pH of 2.0 and 3.0, and decreased to 0.7 mg g −1 as the solution pH increased to 10.0.This result indicated the loading of Fe-Mn oxides improved the removal capacity of sludge biochar for Cr(VI). 13It was not difficult to discover that the removal performance of Cr(VI) by FMBC was stronger on acidic condition.Furthermore, nal pH at adsorption equilibrium on acidic condition was greater than initial solution pH, whereas nal pH was below initial pH on alkaline condition.
The contents of total Cr, Cr(III) and Cr(VI) in residual solution were determined.As solution pH rose from 2.0 to 10.0, the concentrations of total Cr and Cr(VI) rose from 2.84 and 0.83 mg L −1 to 44.79 and 44.79 mg L −1 , respectively, whereas the content of Cr(III) increased from 2.01 mg L −1 to 4.70 mg L −1 and then decreased to under detect limit with increasing solution pH, which indicated that FMBC reduced partial Cr(VI) to Cr(III) (Fig. 2c).More importantly, the Cr(III) concentrations were greater than that of Cr(VI) under acidic condition, while the Cr(III) concentration were very low small or even below the detection value under alkaline condition, which indicated that it was difficult for FMBC to reduce Cr(VI) to Cr(III) on alkaline condition, whereas Cr(VI) ions were adsorbed through adsorption-reduction on acidic condition. 21he concentrations of Fe and Mn in solution aer equilibrium were determined (Fig. 2d).At pH 2.0, the leaching contents of total iron ions were 2.34 mg L −1 , and the contents of total Fe and Fe(III) were substantially comparable, whereas the contents of Fe(II) were small.This was partly due to the fact that Fe(II) will be oxidized by dissolved oxygen, and partly owing to the ability of Fe(II) to supply electron for reducing Cr(VI) and producing Fe(III). 22,23Moreover, the change in Mn concentration decreased gradually with increasing solution pH.To reduce leaching concentrations of Fe and Mn ions and at the same time to ensure Cr(VI) adsorption performance for FMBC, solution pH of 3.0 was selected as the initial pH in subsequent experiments.
To further investigate the inuences of coexisting ions on removing Cr(VI) for FMBC, effects of coexisting cations for Cr(VI) removal were explored (Fig. 2e and f).Na + ions did not have obvious inuence for removing Cr(VI) by FMBC.When concentrations of Ca 2+ and Mg 2+ rose from 0 mg L −1 to 50 mg L −1 , Cr(VI) adsorption performance for FMBC decreased from 93.24% to 92.34% and 91.14%, respectively, which suggested that the presence of Ca 2+ and Mg 2+ exerted a slight inhibitory inuence on removing Cr(VI) for FMBC.However, when the concentrations of Pb 2+ , Cu 2+ and Ni 2+ were increased to 50 mg L −1 , the Cr(VI) adsorption performance for FMBC decreased to 63.68%, 70.32% and 78.96%, respectively.This indicated that there was a serious inhibitory inuences of Pb 2+ , Cu 2+ and Ni 2+ on removing Cr(VI).Among these three heavy metal ions, the inhibitory effect of Pb 2+ was more obvious.According to previous ndings, oxygen-containing group had a much higher affinity for Pb 2+ than the other metal elements.It was also possible that the competitive adsorption of Cr(VI) with Pb 2+ , Cu 2+ and Ni 2+ would compete for active site on FMBC, resulting in decreasing Cr(VI) adsorption performance. 10he inuences of different anions on removing Cr(VI) for FMBC were examined separately (Fig. 3f).SiO 3 2− , NO − 3 and Cl − ions had no signicant inuences on removing Cr(VI) for FMBC when the ions concentrations rose to 50 mg L −1 , and the removal rate was maintained at 93%.Whereas, the co-existence of CO 2- 3 with Cr(VI) produced a slight inhibitory inuences and Cr(VI) removal performance declined to 91.08%.However, there was a signicant inhibitory effect of SO 4 2− and PO 4 3− on removing Cr(VI) for FMBC and the adsorption performance decreased to 75.62% and 68.96%, respectively.This may be due to the fact that sulfate and phosphate ions and HCr 2 O 4 − ions had similar chemical properties, which formed competitive relationship with each other to seize the active sites above FMBC. 9

Adsorption kinetics
The inuences of reaction time for removing Cr(VI) by FMBC are displayed in Fig. 3a.The Cr(VI) removal performance by FMBC increased rapidly from 34.62% to 73.24% within 5-30 min, and Cr(VI) removal performance by FMBC increased to 92.03% at 150 min, and then the removal efficiency stabilized at about 93% and reached equilibrium aer 150 min.This was attributed to the fact that in the rst 30 min, the FMBC surface contained abundant useable active site and can rapidly adsorb Cr(VI) from solution to FMBC surface. 24The useable active site on FMBC surface decreased dramatically during 30∼150 min, which led to slow increase in adsorption performance of Cr(VI) for FMBC.In this stage, Cr(VI) would diffuse from the FMBC surface to the inside pore channels and be adsorbed in active site of inside pore channels. 25The reaction reached equilibrium when all the adsorption sites inside and outside the FMBC were occupied by Cr(VI).The Cr(VI) concentration declined rapidly from 50 mg L −1 to 4.86 mg L −1 in 0-30 min (Fig. 3b).In 30-120 min, the Cr(VI) concentration decreased slowly to 1.38 mg L −1 and Cr(VI) contents remained at about 1.2 mg L −1 aer 120 min.However, the Cr(III) concentrations increased from 0 to 8.52 mg L −1 then decreased to 2.18 mg L −1 , which indicated that the removal behavior belonged to the adsorption-reduction co-action. 26otably, the solution pH (Fig. 3a) rst increased rapidly as the reaction proceeded, and then the solution pH remained around 5.0.Since solution pH affects presence pattern of pollutants and the electrical property of sorbent, the zeta potential value was used to represent the electrical properties of FMBC at different pH, and the result is displayed in Fig. 3c.Potentiometric analysis expressed that zeta potential value of FMBC shied from positive to negative with the increase of pH, indicating that electrical property of FMBC shied from positive to negative electricity. 10The zero potential point (pH pzc ) of FMBC was 3.74.In aqueous solution, Cr(VI) exists mainly as the anion HCr 2 O 4 − at solutions pH < 6.0, while Cr(III) exists as Cr 3+ . 27This suggested that in the early stage of reaction, the positively charged FMBC adsorbed Cr(VI) to the surface by electrostatic action, and then reduced Cr(VI) to cation Cr(III) by reducing substance, and due to electrostatic repulsion Cr(III) ions were released to aqueous solutions. 28During the Cr(VI) reduction, there were a continuous consumption of H + in the solution, which was the reason for the increase in pH.When solution pH outweighed pH pzc , FMBC adsorbed the cation Cr(III) in solutions to surface by electrostatic action.Notably, the change in solution pH was mainly concentrated within 30 min, indicating that reduction reaction of Cr(VI) for FMBC was mainly concentrated in early stage of removal process.
To research removal process of Cr(VI) for FMBC, the pseudo rst order kinetic model, pseudo second order kinetic model and Elovich model were chosen to describe the experiment results, and tting result is displayed in Fig. 4a and Table 1.The linear correlation coefficient of pseudo second order kinetic model (R 2 = 0.997) was higher than that of pseudo rst order kinetic model (R 2 = 0.967) and Elovich model (R 2 = 0.941).Additionally, the difference between the theoretical adsorption capacity (q e,cal ) obtained from pseudo rst order kinetic model (114.00mg g −1 ) and the actual adsorption capacity (q e,exp , 116.48 mg g −1 ) was large, whereas the difference between the tted value from pseudo second order kinetic model (117.22 mg g −1 ) and the q e,exp was small, which indicated that the pseudo second order kinetic model could better describe the Cr(VI) removal for FMBC than the pseudo rst order kinetic model. 29his expressed that the removal behavior of Cr(VI) for FMBC was mainly controlled by chemisorption. 30Briey, the Cr(VI) removal behavior by FMBC was primarily controlled through chemical effects (e.g., complexation and electron transfer), while physical effects (e.g., electrostatic effects and pore lling) were secondary to controlling the reaction process. 5,12rdinarily, diffusion behavior in removal process is determined by multiple mechanism.The intra-particle diffusion model and the liquid lm diffusion model were employed to nd out the diffusion behavior and the rate control steps.The curves of q t over t 1/2 consisted of three linear segments (Fig. 4b), indicating that Cr(VI) removal behavior by FMBC had multiple stage. 9In general, three stages were divided into external diffusion, internal diffusion and adsorption equilibrium.The curve of external diffusion stage had high slope (K d1 ), indicating Cr(VI) ion in solutions transferred to outer surface.The second part of diffusion trend slowed down signicantly and belonged to the internal diffusion phase, where Cr ions diffused from the external surface into the structure of FMBC and were subsequently adsorbed to internal adsorption site. 23The third part was equilibrium stages.Additionally, the C i values (Table S2 †) for all stages showed a tendency to deviate from 0, suggesting that intra-particle diffusion was not the only controlling factor in removal processes. 31Moreover, the intra-particle diffusion constants showed K d1 > K d2 > K d3 , and the boundary layer constants showed C 1 < C 2 < C 2 , which showed that external diffusion dominated the removal behavior. 10The outcome of lm diffusion is displayed in Fig. 4c and Table S2.† The outcome indicated that liquid lm diffusion diagram held linear relationship, and R 2 value (0.990) kept at a high level, which indicated that the liquid lm diffusion played a decisive role in the kinetic process. 9Briey, the removal behavior can be divided into the following step: liquid lm diffusion rst controlled adsorption behavior by removing Cr(VI) from liquid phase to outer surface of FMBC; then the entire removal processed were determined by intra-particle diffusion, and Cr(VI) entered into the inner pore structure and loaded into internal active sites until adsorption saturation.

Adsorption isotherm
The Cr(VI) adsorption performance for FMBC rose rapidly as Cr(VI) concentration rose from 50 mg L −1 to 100 mg L −1 , which attributed to large Cr(VI) concentrations difference between solutions and FMBC, which created large mass-transfer resistance and allowed Cr(VI) to be adsorbed onto FMBC surface.However, the Cr(VI) adsorption performance by FMBC did not change much as concentration rose from 100 mg L −1 to 150 mg L −1 , because active sites on FMBC surface were limited. 29o further understand the properties of the adsorption, four commonly isotherm models (Langmuir, Freundlich, Temkin and Sips models) were used in this work, and the result is shown in Table 2 and Fig. 4d.The R 2 (0.992-0.996) value of Langmuir model was signicantly greater than Freundlich

Fitting result
Experimental data q e,exp (mg g −1 ) 116.48 Pseudo-rst-order q e,cal (mg g −1 ) 114.00 k 1 (min −1 ) 0.086 R 2 0.967 Pseudo-second-order q e,cal (mg g −1 ) 117.22 k 2 (g mg −1 min −1 ) 0.001 R 2 0.997 Elovich a (mg g −1 min −1 ) 66.723 b (g mg −1 ) 0.057 R 2 0.941 model (0.752-0.867),Temkin model (0.934-0.966) and Sips model (0.924-0.961), which indicated that Cr(VI) adsorption processes for FMBC were homogeneous monolayer adsorption. 32Additionally, the results of chi-square test (c 2 ) showed that Langmuir model could better describe Cr(VI) removal process for FMBC than the Freundlich, Temkin and Sips model. 12The separation factor (R L ) of Langmuir model remained between 0 and 1 (Fig. S4a †), suggesting that Cr(VI) removal by FMBC was effective. 10Meanwhile, elevated temperature reduced the R L value, which indicated that high temperature could promote Cr(VI) removal for FMBC. 10 According to Langmuir model, the largest theoretical removal performance of FMBC at 303 K was 172.34 mg g −1 .Temkin model (R 2 > 0.93) well described the experimental results, suggesting that there was strong intermolecular force between Cr in solution and the FMBC surface, which may be involved in the redox action and complexation.
Based on the Van't Hoff equation, the ln K 0 was used to plot 1/T (Fig. S4b †), and the slope and intercept of obtained straight line were used to calculate the value of DH 0 and DS 0 , and then the value of DG 0 was calculated (Table 3).The DH 0 was greater than 0, which indicated that the removal reaction was a heatabsorbing reaction. 9The negative value of DG 0 decreased with increasing temperatures, demonstrating that Cr(VI) removal behavior for FMBC was spontaneous. 16DS 0 was positive, suggesting that Cr(VI) removal processes for FMBC were entropydriven, and degree of freedom at solid-liquid interface increased during removal process. 20

Reduction-adsorption mechanism
The morphological features and surface element of FMBC were analyzed by SEM-EDS (Fig. 5a and b).Aer adsorption, the uneven surface became rougher than before adsorption and massive small particles were attached, which may be due to that Cr adsorbed on FMBC surface.According to the mapping pattern of EDS, elemental Cr appeared on the FMBC surface aer adsorption, which demonstrated that Cr in the aqueous solution was successfully removed by FMBC.The crystalline structure (Fig. 5c) of FMBC before and aer removal remained basically unchanged, and the main components were SiO 2 and CaAl 2 Si 2 O 8 . 33,34However, the characteristic peaks of MnFe 2 O 4 at 29.86°, 35.14°and 61.92°showed different degrees of decrease aer adsorption, which could be the involvement of MnFe 2 O 4 in Cr(VI) removal from aqueous solution.
To further illustrate mechanisms of Cr(VI) adsorption for FMBC, the functional groups of FMBC were analyzed by FTIR (Fig. 5d).Aer removal, the wavenumber of hydroxyl group -OH at 3390 cm −1 in FMBC shi to 3420 cm −1 , and the intensity of -OH vibrational peaks was weakened.Notably, the intensity of vibrational peaks of -COOH group, C-O group and Mn/Fe-O group in FMBC were all weakened or shied aer adsorption.Most notably, the wavenumber of the -COOH group shied from 1400 cm −1 to 1380 cm −1 aer the adsorption, and the intensity of the vibrational peak of the -COOH group also underwent a signicant weakening.The wavenumber of C-O group was offset from 1040 cm −1 to 1030 cm −1 .In addition, the vibrational peak of Mn/Fe-O group could be observed to be offset from 539 cm −1 to 526 cm −1 and the intensity of the peak appeared to be slightly reduced, which could be due to the reduction caused by the dissolution of the Mn or Fe elements in FMBC.These results indicated that the oxygen-containing groups (e.g., -OH, -COOH, C-O, and Mn/Fe-O groups) on the FMBC complex with negatively charged Cr(VI). 13,25,35Notably, the vibrational peak of C]C groups at 1640 cm −1 was shied to 1610 cm −1 , where the vibrational peaks were attributed to the C]C group on the carbon ring, which could be able to provide p-electrons as the adsorption site for contaminants and remove contaminants from solution by cation-p interactions. 32owever, since Cr(VI) existed mainly as anion in solution, this could be the result of cationic-p interaction between Cr(III) generated by reduction and C]C structure on FMBC during the adsorption process. 20According to the previous ndings, the C]C group shied from 1640 cm −1 to 1610 cm −1 aer Cr(VI) removal from solution, which was also consistent with the present study. 1,22These analysis showed that FMBC adsorbed Cr(VI) on surface through complexation and electrostatic interactions, and Cr(VI) ion was reduced to cationic Cr(III), and then released cation Cr(III) into solutions by electrostatic repulsion.When solution pH outweighed zero potential point of FMBC, the negatively charged FMBC adsorbed the positively charged Cr(III) from the solution in the form of Cr(III)-p interaction, complexation and electrostatic interaction.
To gain deeper understanding of adsorption mechanism of Cr(VI) for FMBC, the sample before and aer removal was analyzed through XPS.Fig. 6a showed full spectrum of FMBC before and aer Cr(VI) adsorption, and Cr 2p peaks were detected on the full spectrum aer the removing Cr(VI), suggesting that Cr(VI) ions were successfully adsorbed in FMBC surface.The peak of Cr(III) and Cr(VI) appeared in Cr 2p 3/2 ne spectra (Fig. 6b), further indicating that Cr(VI) ions were reduced to Cr(III) by FMBC.The Cr(III) and Cr(VI) peaks correspond to binding energies of 576.88 eV and 578.30eV, respectively, the percentage of Cr(III) and Cr(VI) was 72.77% and 26.23%, respectively.This result indicated that the vast majority of Cr(VI) was removed through adsorption-reduction. 24,28 The primary peak of O 1 s before removal in Fig. 6c were Mn/Fe-O (529.51 eV), C-O (530.71eV) and C]O (531.66 eV). 10,19,36The decreasing peak areas of Mn/Fe-O/C-O and increasing peak area of C]O indicated that FMBC could be used as electrons transfer medium and attend reactions through the gain and loss of electron by O-containing functional group. 3In addition, binding energy of C-O and C]O appeared to increase aer the reaction, which was presumed to be due to the O-containing groups in FMBC complexing with Cr(VI). 23In N 1 s spectra (Fig. 6d), the peaks were N-C (398.28 eV), N-H (399.58 eV) and N-O (402.20 eV). 3 Aer Cr(VI) removal, the binding energy of N-C, N-H and N-O groups shied to 398.50 eV, 400.03 eV and 402.70 eV, respectively, suggesting that chemical reaction between the N-containing groups in FMBC and Cr(VI) took place. 3Previous literature demonstrated the ability of N-C groups in biochar to provide lone pair electrons for coordination reactions with Cr(VI). 37Moreover, previous literature had also shown that the N-H group in biochar could act as an electron donor triggering an electron transfer reaction to facilitate the reduction of Cr(VI). 38The Fe 2p spectra (Fig. 6e) were roughly classied into Fe(II) and Fe(III), and the relative amount of Fe(II) was reduced from 44.74% to 29.78% aer the reaction, while the content of Fe(III) in FMBC increased from 55.26%.This result indicated that Fe(II) in FMBC could reduce Cr(VI) to Cr(III). 32Similarly, in Mn 2p spectrum (Fig. 6f), the content of Mn(II) decreased from 64.28% to 60.50% aer the reaction, which also indicated the redox reaction between Mn(II) and Cr(VI). 19The result demonstrated that Mn and Fe in FMBC could reduce Cr(VI) to Cr(III).Meanwhile, the binding energies of both Mn and Fe shied to higher energy levels aer reaction, which further conrmed that Mn and Fe played a key role in removing Cr(VI).
Anionic Cr(VI) in solutions was adsorbed to FMBC surface by complexation containing N/O groups or electrostatic interaction, and Cr(VI) ions on FMBC surface were reduced to positively charged Cr(III) by reducing substances in FMBC (e.g., divalent iron/manganese or reduced phenolic hydroxyl groups).The resulting cation Cr(III) with the positively charged FMBC would undergo electrostatic repulsion and be released into the aqueous solution.Notably, the reduction reaction continued to consume massive H + in the aqueous solutions.When solutions pH was higher than pH pzc , Cr(III) in the aqueous solution could be adsorbed onto the FMBC surface through the complexation of N/O groups, electrostatic interactions, and cation-p interactions.

Performance in treating Cr(VI)-containing wastewater
To explore practicality, the FMBC was employed to remove Cr(VI) from electroplating wastewater (Fig. 7a) and mineral dissolving wastewater (Fig. 7b).At dosage of 0.4 g L −1 , Cr(VI) concentration in both water samples decreased rapidly and the residual Cr(VI) contents were higher than 0.2 mg L −1 , and this result did not meet the discharge standard for Cr(VI)-containing wastewater (0.2 mg L −1 ).To increase the removal rate, the dosage of FMBC was increased to 1 g L −1 , and FMBC was able to remove Cr(VI) to less than 0.2 mg L −1 (Chinese Cr(VI) emission standard) in both electroplating wastewater and mineral dissolving wastewater at 90 min and 30 min, respectively, which indicated that FMBC had potential to be applied to the treatment of real wastewater.

Regeneration experiment
Aer each adsorption, the FMBC in aqueous solution was separated by magnet, then the adsorbed FMBC was regenerated by shock desorption for 12 h.In Fig. 7c, removal efficiency of Cr(VI) by FMBC declined with increasing number of regenerations when Cr(VI) contents were 50 mg L −1 .However, Cr(VI) removal performance by FMBC was still 82.34% in the h regeneration.When Cr(VI) contents were declined to 5 mg L −1 (Fig. 7d), the Cr(VI) removal efficiency for FMBC was still as high as 97.68% aer ve regenerations.This result indicated that

Conclusion
In this research, Fe-Mn oxide loaded sludge biochar (FMBC) was prepared.The Cr(VI) removal processes for FMBC were in accordance with pseudo-second-order kinetic and Langmuir model, and largest removal performance of FMBC for Cr(VI) was 172.34 mg g −1 .Additionally, the Cr(VI) adsorption processes for FMBC were a spontaneous, monolayer and homogeneous chemical adsorption, and held obvious pHdependent.Removing Cr(VI) mechanism for FMBC involved Cr(VI) adsorption-reduction, and the re-absorption process of Cr(III) generated by reduction.FMBC showed excellent performance in removing Cr(VI) from electroplating wastewater and mineral dissolving wastewater.Additionally, FMBC was regenerated at least ve times and effectively remove Cr(VI) in wastewater.

Fig. 2
Fig. 2 Influence of solution pH on removing Cr(VI) for FMBC and solution pH after adsorption equilibrium (a), correlation between solution pH and adsorption capacity (b), and the content of Cr, Fe and Mn in solution after adsorption equilibrium ((c) Cr and (d) Fe and Mn).Effect of coexisting cation (e) and co-existing anion (f) on Cr(VI) removal by FMBC.

Fig. 3
Fig. 3 Influences of adsorption time on removing Cr(VI) for FMBC and change of solutions pH (a), influences of adsorption time on Cr concentration in solution (b) and analysis of zeta potential value of MFBC (c).

Fig. 4
Fig. 4 The kinetic models for removing Cr(VI) by FMBC ((a) pseudo-first-order, pseudo-second-order and Elovich, (b) intra-particle diffusion model and (c) liquid film diffusion model) and the adsorption isotherm for removing Cr(VI) by FMBC at different temperature (d).

Fig. 5
Fig. 5 The result of SEM-EDS (a and b), FTIR (c) and XRD (d) analysis for Cr(VI) removal by FMBC.

Table 2
Adsorption isotherm fitting parameter of removing Cr(VI) for FMBC

Table 3
Thermodynamic fitting parameter of removing Cr(VI) for FMBC